A new magnesium sheet alloy with high tensile properties and room-temperature formability

Lightweight sheet alloys with superior mechanical performance such as high strength, ductility and formability at room temperature (RT) are desirable for high volume automotive applications. However, ductility or formability of metallic alloys at RT are generally inversely related to strength, thereby making it difficult to optimize all three simultaneously. Here we design a new magnesium sheet alloy-ZAXME11100 (Mg-1.0Zn-1.0Al-0.5Ca-0.4Mn-0.2Ce, wt. pct.) via CALPHAD (CALculation of PHAse Diagram) modeling and experimental validation. This new sheet alloy offers an excellent RT formability with a high Index Erichsen (I.E.) value of 7.8 mm in a solution-treated condition (T4), due to its weak and split basal texture and fine grain structure. The new ZAXME 11100 alloy also shows a rapid age-hardening response during post-forming artificial aging treatment at 210 °C for 1 hour (T6), resulting in a significant increase of yield strength from 159 MPa (T4) to 270 MPa (T6). The excellent combination of T4 ductility (31%), T4 formability (7.8 mm) and T6 yield strength (270 MPa) in this new magnesium alloy is comparable to that of common 6xxx series aluminum sheet alloys. Thus, this new magnesium sheet alloy is highly attractive for sheet applications in automotive and other industries.

www.nature.com/scientificreports www.nature.com/scientificreports/ of Phase Diagrams) modeling [24][25][26][27] , as a part of Integrated Computational Materials Engineering (ICME) 28 framework, has been successfully applied to study the alloying-processing-structure-property relationships in multicomponent alloy systems. Therefore, CALPHAD simulation is used to design a new Mg-1Zn-1Al-0.5Ca-0.4Mn-0.2Ce alloy (hereafter designed as ZAXME11100) and its optimal TMP to obtain more balanced strength, ductility and formability in this study. TMP (including homogenization, rolling and annealing) is critically important in optimizing the alloying effects for the final mechanical properties of the alloy. For example, conventional homogenization process (at below solidus temperature of the alloy to avoid incipient melting) is inefficient in dissolving second phases from the as-cast microstructure and maximizing the solute concentrations in the Mg matrix, thus achieving the overall alloying effects.
In this paper, CALPHAD simulation is used to design a new homogenization process (with multiple isothermal stages including final stages at temperatures higher than the alloy solidus 18 ) for the new alloy, achieving maximum dissolution of alloying elements without incipient melting. The combination of the new alloy design and the multi-stage TMP process leads to the optimum combination of strength, ductility and formability of the new alloy.

Results and discussions
CALPHAD software Thermo-Calc and TCMG5 and MOBMG1 databases 29 was used to perform the thermodynamic and kinetic modeling of ZAXME11100 alloy. Figure 1(a) shows the solidification path of ZAXME11100 alloy using the classical Scheil model, and an enlarged region near the end of solidification is shown in Fig. 1(b). The results show that HCP (hexagonal closed packed) Mg phase will form as a primary phase at 638 °C, followed by the formation of Al 8 Fig. 1(c), which are slightly higher than those (628 °C and 546 °C, respectively) of the same phases during cooling (solidification) in Fig. 1(a,b). Similarly, the formation of Al 2 Ca, Ca 2 Mg 5 Zn 5 and Al 11 Mn 4 is at 430 °C, 172 °C, and 208 °C, respectively, which is considerably lower than their temperatures (488 °C, 368 °C, and 329 °C) of formation during solidification in Fig. 1(a,b). On the other hand, Ce 2 Mg 53 Zn 45 and Ca 2 Mg 5 Zn 13 phases formed during solidification in Fig. 1(b) are not shown in the equilibrium calculation in Fig. 1(c), thus they are assumed to be metastable phases.
Based on these results, a new homogenization profile (designated as H480, thereafter) was designed with four isothermal stages (320 °C for 4 h, 360 °C for 4 h, 440 °C for 52 h and 480 °C for 1 h) to sequentially dissolve the intermetallic phases while avoiding incipient melting. The first stage was designed as 320 °C between the formation temperatures of stable phases (Ca 2 Mg 5 Zn 5 at 172 °C; and Al 11 Mn 4 at 208 °C) in Fig. 1(c) and the solidified phases (Ca 2 Mg 5 Zn 5 at 368 °C; and Al 11 Mn 4 at 329 °C) in Fig. 1(b), to initially dissolve the stable phases (Ca 2 Mg 5 Zn 5 and Al 11 Mn 4 ) and the metastable phases (Ce 2 Mg 53 Zn 45 and Ca 2 Mg 5 Zn 13 ). The second stage was www.nature.com/scientificreports www.nature.com/scientificreports/ done at 360 °C for 4 h to further dissolve the phases with higher melting temperatures, such as Ca 2 Mg 5 Zn 5 phase (368 °C) in Fig. 1(b) and also reduce the micro-segregation of alloying elements.
The third stage was carried out at 440 °C for 52 h between the formation temperature of Al 2 Ca (430 °C) in Fig. 1(c) and (488 °C) in Fig. 1(b), to dissolve Al 2 Ca phase and further homogenize the alloying elements. Figure 1(c) shows a small fraction of liquid at temperatures above the solidus 450 °C. Also, a new phase AlCaMg would possibly form during this stage since it is thermodynamically stable between 430 °C and 478 °C in Fig. 1(c). Thus, the fourth stage was chosen as 480 °C for 1 h to dissolve AlCaMg and potentially Mg 12 Ce and Al 8 Mn 5 phases with higher thermal stability up to 548 °C and 632 °C, respectively. However, the liquid phase was not experimentally observed during the fourth stage (480 °C, 1 h). The reason could be: (1) the homogenization time was not long enough for the liquid phase to form; or (2) the amount of the liquid phase formed was too small (<~1%, 480 °C in Fig. 1(c)). Thus, the multi-stage homogenization profile (H480) and rolling process (R450) used in producing the ZAXME 11100 alloy sheet are summarized in Fig. 1(d).
Diffusion-controlled distribution of solutes Al, Zn, Ca, Ce and Mn in Mg matrix was studied using DICTRA 29 simulation, and Fig. 2(a) plots the calculated solute distributions in both the as-cast (AC) condition and the new H480-homogenized condition. The results demonstrate that the new multi-stage treatment is very effective in dissolving solute elements in Mg grain interiors. Figure 2(b) shows that the diffusion coefficients of Al, Zn, Ca, Mn and Ce solutes in ZAXME11100 alloy are exponentially related to temperature. For example, the diffusion coefficients of the solutes at 480 °C are about 10 times higher than those at 400 °C close to the solidus temperature (450 °C), suggesting that significantly faster homogenization is possible at 480 °C compared to 400 °C (which is below the 450 °C solidus temperature). It is also noted that Al and Mn have the lowest diffusion coefficients www.nature.com/scientificreports www.nature.com/scientificreports/ among all alloying elements in Mg, which also explains that Al 8 Mn 5 is the most difficult phase to be dissolved during solution treatment.
Microstructures of ZAXME11100 alloy after as-cast condition and the new homogenization treatment (H480) were observed via optical microscopy and shown in Fig. 2(c,d), respectively. The results showed that the second phase particles near and along the grain boundaries have been essentially dissolved after the new homogenization profile (H480). However, a small amount of residual particles, mostly Al 8 Mn 5 and a very few Al 2 Ca as identified in TEM, are still visible in Fig. 2(d).
The new Mg alloy solutionized at H480 heat treatment has been rolled following the designed rolling process (R450) in Fig. 1(d). The grain size of microstructure from as-cast (AC), H480 and as-rolled (AR) conditions is shown in Fig. 3. It should be noted that (1) the grain size at H480 solution treatment has slightly grown to 312.3 μm, which could be attributed to the inhibition of thermally stable Al 8 Mn 5 and Al 2 Ca particles formed during the solidification; and (2) the grain size has been significantly decreased to 4.7 μm at as-rolled condition due to recrystallization of the deformed microstructure.
The EBSD inverse pole figure (IPF) map overlaid by large angle grain boundaries with misorientation angles larger than 15 degrees in Fig. 4(a) shows the microstructure of ZAXME11100 alloy after rolling process (R450) followed by the post-forming solution treatment (T4) and water quenching from Fig. 1(d). The average grain size of ZAXME11100 alloy determined via EBSD is about 9.6 μm. It can be seen that the combination of rolling (R450) with the post-forming solution-treatment (T4) yields significant grain refinement in ZAXME11100 alloy. The texture pole figures of solution-treated (T4) microstructure are shown in Fig. 4(b). The microstructure has a weak split basal texture with a maximum intensity of 3.3 mrd. The maximum intensity of basal poles is also tilted by about ±40 degrees away from the normal direction (ND) and toward the transverse direction (TD). Such fine grain size and weakened texture of solution-treated (T4) ZAXME11100 sheet alloy contribute to both high ductility and formability 11,14 .
The high-angle annular dark-field (HAADF) STEM image in Fig. 5(a) shows a high density of intermetallic particles in the post-forming T4 microstructure. STEM energy dispersive spectroscopy (EDS) elemental maps were collected from the region showing in Fig. 5(a). The STEM-EDS elemental maps in Fig. 5(b-f) show that the nano-scale rod precipitates are enriched with Al and Mn elements. Elements Zn, Ca and Ce (not shown in Fig. 5 due to small amount) are homogeneously distributed in the grain interior, suggesting that those alloying elements are dissolved in Mg matrix, hypothesized to form solute co-clusters 11,12 during subsequent aging heat treatments and thereby contribute to strengthening of the ZAXME11100 alloy. www.nature.com/scientificreports www.nature.com/scientificreports/ Bright-field (BF) STEM image in Fig. 6(a) reveals that the T4 microstructure consists of a high density of uniformly distributed nano-size rod precipitates randomly distributed both within grain interior and at grain boundaries. Bright field (BF) TEM image with an inset selected diffraction patter in Fig. 6(b) shows that the rod precipitates are Al 8 Mn 5 phase. As shown in Fig. 1(b,c), Al 8 Mn 5 starts to form at 628 °C during solidification and melt at 632 °C under the post-heat treatment. It cannot be dissolved during solution treatment at 480 °C. Therefore, Al 8 Mn 5 can retard grain growth through Zener pinning during annealing at 480 °C, thus contributing to grain refinement. High density and uniformly distributed Al 8 Mn 5 phase also contribute to the strength of T4 microstructure. Figure 7(a) shows the variation in the Vickers hardness of solution-treated (T4) ZAXME11100 sheet alloy under the artificial aging at 210 °C. The ZAXME11100 sheet alloy has a hardness value of 56.0 ± 2.1 HV in the  www.nature.com/scientificreports www.nature.com/scientificreports/ solution treated condition (T4) from Fig. 1(d) and exhibits a rapid age-hardening to a peak hardness of 70.8 ± 1.5 HV for 1 h. The tensile curves obtained from solution-treated (T4) and peak-aged (T6) samples are shown in Fig. 7(b). The mechanical properties of these samples are summarized in Table 1 Figure 7(c,d), respectively, summary the engineering  www.nature.com/scientificreports www.nature.com/scientificreports/ stress as a function of I.E. values as well as engineering strain for various Mg 8,11,12,14,[30][31][32][33][34] and Al 35,36 sheet alloys. As can been seen, the ZAXME11100 sheet alloy shows good stretch formability in T4 condition, which is close to that reported for 6000 series Al alloy 35,36 . Subsequently the artificial aging (T6) treatment substantially increases the engineering stress with less reduction of ductility, enabling this alloy to have a well-balanced high strength, ductility and formability at room temperature.
The preliminary STEM imaging in Fig. 8(a,b) for the T6 microstructure of ZAXME11100 alloy did not reveal the formation of crystalline precipitate phases, except for the nano-size Al 8 Mn 5 rods which were seen previously in the solution-treated samples (Fig. 6). This suggests that solutes Al and Mn have the strongest affinity in the ZAXME11100 alloy and that other solutes may not have enough strong affinity to form crystalline phases during aging. Figure 8 Table 1. Mechanical properties of ZAXME11100 sheet alloy at room temperature. www.nature.com/scientificreports www.nature.com/scientificreports/ (−15521.2 J/mol) pairs are significantly negative. Therefore, thermodynamically, there is a strong affinity between the corresponding solutes to form solute clusters or crystalline phases. It should be noted that the Al-Mn pair has the most negative enthalpy of mixing, suggesting that solute pair Al and Mn has a much stronger affinity than other solute pairs, and therefore is most likely to form crystalline precipitates.
Based on results from Fig. 8(a-c), the Al-Mn atomic pair with strongest affinity would form crystalline Al 8 Mn 5 phase. Other atomic pairs with negative mixing enthalpies may form some clusters 11,12 without forming distinct observable precipitates during the ageing treatment. Further characterization work is on-going to investigate the strengthening mechanism involved in T6 treatment. Therefore, the significant enhancement of engineering strength after T6 treatment would be attributed to the formation of solute clusters 11,12 in Fig. 8(d), which should provide a string pinning effect on the basal <a> dislocations. These dislocations need a larger force to break away from the solute atmosphere after aging (T6). Therefore, the combination of designing new alloy and optimizing TMP with CALPHAD methodology has led to a heat-treatable magnesium sheet alloy (ZAXME11100) with excellent RT-formability and high strength, which has overcome the well-known strength-formability dilemma.

conclusions
In summary, a new Mg sheet alloy (ZAXME11100: Mg-1Zn-1Al-0.5Ca-0.4Mn-0.2Ce) and a novel thermomechanical process have been developed based on CALPHAD and diffusion modeling in combination with experimental investigation. The new Mg sheet alloy produced via low-cost rolling followed by a multi-stage solution treatment (T4) and conventional aging treatment (T6) has a superior combination of high strength (270 MPa in T6), ductility (31% in T4) and formability (Erichsen Index of 7.8 mm in T4) at room temperature. Microstructure characterization and thermodynamic/kinetic calculations suggest that the following factors contribute to the excellent properties: (1) weak and split basal texture; (2) fine grain structure (average 9.6 μm); and (3) possible formation of solute clusters after a short-time aging treatment (T6) due to the negative mixing enthalpy of various solute pairs. The new ZAXME11100 sheet alloy has successfully overcome the common trade-off relationship between formability/ductility and strength, promising high-volume automotive applications of magnesium sheet components.

Materials and methods
Magnesium sheet alloy preparation method was reported in a previous publication 18 . Mg-1Zn-1Al-0.5Ca-0.4Mn-0.2Ce (ZAXME11100) alloy was prepared in a steel crucible under a protective gas mixture of CO 2 and SF 6 , then cast at 750 °C into a steel mold pre-heated to 400 °C to produce 110 × 114 × 18 mm plates. The cast plates were machined into 20 × 28 × 7 mm samples which were homogenized (multi-stage H480) and water-quenched. The homogenized samples were cold-rolled initially to ~3 mm with about 0.25 to 0.5 mm thickness reduction per pass, and then rolled to ~1 mm with 30% thickness reduction per pass. Except for the final rolling pass, the samples were pre-heated at 450 °C for 5 min prior to each pass. Longitudinal tensile samples with a gauge length of 12.5 mm, a width of 5 mm, and a thickness of 1 mm were machined from the as-rolled sheets. Some as-rolled tensile samples were solution-treated at 480 °C for 1 h (T4) followed by water-quenching and then artificial aging at 210 °C for 100 hours in an oil bath. Age hardening responses of the solution-treated samples were measured using a Vickers hardness tester. Tensile tests were conducted at RT on the solution-treated (T4) and peak-aged (T6) samples at a strain rate of 1.8 × 10 −4 s −1 . At least three specimens were tested at RT for each temper condition to ensure repeatability. To evaluate the stretch formability of the solution-treated (T4) sheets, Erichsen cupping tests were performed at RT on 60 × 60 mm rectangular samples with a thickness of 1 mm using an Erichsen sheet metal testing machine with a 20 mm diameter hemispherical punch. The punch speed and blank-clamping force were around 6 mm/min and 10 kN, respectively. Graphite lubrication was used on the tool.
The microstructure of the new alloy was characterized using optical microscopy, scanning electron microscopy (SEM), transmission electron microscopy (TEM) and scanning transmission electron microscopy (STEM). The SEM study and electron backscatter diffraction (EBSD) mapping were conducted using a FEI Apreo SEM equipped with a EDAX OIM system. Specimens for TEM analysis were mechanically ground to ~40 μm using a Fischione model 100 dimpler. Perforation of thin TEM foils were conducted in a Fischione model 1010 ion mill operating at a voltage of 5 keV. TEM and STEM investigations were carried out on a FEI Tecnai F20 TEM/STEM microscope operating at 200 kV. STEM-EDS elemental maps were collected using a FEI G2 60-300 TEM/STEM microscope equipped with a Super-X/ChemiSTEM) EDS system operating at 300 kV.